{'fraction_non_alphanumeric': 0.040972935936964716, 'fraction_numerical': 0.025693730729701953, 'mean_word_length': 4.448301605076521, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Ionic-exchange immobilization of ultra-low loading palladium on a rGO electro-catalyst for high activity formic acid oxidation

A formic acid oxidation electro-catalyst with ultra-low palladium (Pd) loading was prepared via an ionic exchange method by utilizing the acidic functional groups on graphene oxide (GO). After simultaneous reduction of exchanged Pd2+ and residual functional groups on the GO surface, an ionic exchange reduced Pd catalyst supported on reduced GO (IE-Pd/rGO) was obtained. Three times improved formic acid oxidation mass activity compared with that of the conventional synthesized Pd/C catalyst was exhibited for the IE-Pd/rGO catalyst. More importantly, formic acid oxidation stability on the IE-Pd/rGO catalyst was remarkably improved due to synergistic effect of the strong immobilization of Pd nanoparticles and the effect of in situ doped N on the rGO support.


Introduction
Formic acid (FA) has been considered as one of the most potential alternative liquid fuels to replace methanol in direct liquid fuel cells due to the much faster kinetics of the FA oxidation reaction (FAOR) than that of the methanol oxidation reaction [1][2][3][4] and much lower fuel crossover rate through the proton exchange membrane. 5,6 Despite the development on Pt based FAOR catalysts, 7-10 noble metal palladium (Pd) electrochemical catalysts [11][12][13] are required for FA oxidation catalysis to achieve satisfactory power output of the direct formic acid fuel cell (DFAFC). [14][15][16][17][18][19][20][21][22] Other than the high cost of Pd, poor FAOR stability on Pd catalyst is also an important issue strongly hinders the practical application of DFAFC technology. 23,24 In order to overcome this stability issue, numerous strategies were carried out to alter the FAOR process or to improve the efficiency of single Pd active sites. 25,26 Among these strategies, doping a second metal with Pd to change the FAOR process is the most commonly used one. [27][28][29][30] Due to the electron effect 31 or the third-body effect, 32,33 generation of Pd poison intermediates can be suppressed. Most mechanism studies claimed that continuous Pd active sites should be isolated no matter what the poison intermediate was. [34][35][36] An alternative strategy is to stabilize the Pd nanoparticles isolated during the DFAFC operation. 36 The best route to stably isolate the Pd nanoparticles is mono-dispersing the nanoparticles on graphene, 37-39 which has been widely studied as catalyst support 40 due to the great electronic conductivity and abundant surface functional groups on graphene oxide (GO). [41][42][43] Plenty of Pd/graphene catalysts were therefore developed with improved FAOR catalytic performance than the conventional Pd/C catalysts. 44,45 However, Pd loading in the reported Pd/graphene catalysts is still high. 39 In the present work, a novel route ( Fig. 1) was proposed to synthesis highly active Pd loaded reduced GO (rGO) catalyst with ultra-low palladium loading. Acidic functional groups, including -COOH and -SO 3 H, generated on GO surface was used for Pd 2+ exchange during this ionic-exchange assisted synthesis process. The exchanged Pd 2+ on GO surface was subsequently in situ reduced together with the residual oxidation functional groups, e.g. -OH and NO 2 groups. Pd nanoparticles were therefore stably anchored on rGO to produce an ionic exchange assisted Pd/rGO (IE-Pd/rGO) catalyst. The IE-Pd/ rGO catalyst exhibited great catalytic efficiency and stability for FAOR compared with the conventional prepared Pd/C catalyst. As a result, with only ca. 7 wt% Pd loaded, the IE-Pd/rGO FAOR catalyst performed much better than the conventional Pd/C with more than 20 wt% Pd loaded in terms of both electrochemical oxidation current and stability.

Experimental
2.1. Catalyst synthesis 2.1.1. IE-Pd/rGO catalyst. GO was prepared from oxidation of powdered ake graphite using the modied Hummers' method. 46 The exchange of Pd 2+ ions of the functionalized GO was achieved by dispersing GO (0.1 g) in deionized water (50 mL). Subsequently, palladium acetate (45 mmol) was added into the dispersion and the mixture was treated in an ultrasonic bath for 30 min. The mixture was then magnetically stirred overnight for Pd 2+ exchange. Despite the low solubility of palladium acetate in water, ionic exchange would take place completely due to the continuously consumption of palladium acetate. The Pd 2+ exchanged GO sheets were dried at 40 C for 12 h in vacuum oven subsequent to washing with deionized water and acetone for several times. Simultaneously reduction of Pd 2+ and oxygen-contained groups on the Pd 2+ /GO sheets were carried out by adding excessive hydrazine hydrate (85% N 2 H 5 OH aqueous solution) into 40 mL Pd 2+ -GO solution. Aer being stirred overnight, the black slurry was ltered, washed and dried at 60 C. The product was denoted as IE-Pd/rGO for further use.
2.1.2. IR-Pd/C catalyst. The Pd/C catalyst for comparison was prepared by conventional impregnation reduction method and denoted as IR-Pd/C catalyst. 47 100 mg Vulcan XC-72 carbon black and 10 mL H 2 PdCl 4 (2.5 mg mL À1 ) solution were dispersed uniformly in 100 mL of deionized water with vigorously stirring for 1 h. 15 mL freshly prepared 20 mM cetyltrimethyl ammonium bromide (CTAB) solution, 5 mL 50 mM ascorbic acid solution and 5 mL 0.5 M NaOH were added into the mixture in sequence with magnetic stirring. Aer reaction overnight, the solution was ltered, and thoroughly washed by hot deionized water to get rid of CTAB. Finally, the catalyst was dried at 60 C and was ground into a ne powder state.

Characterization
Powder X-ray diffraction (XRD) analyses were performed on a Bruker D8-FOCUS Advance diffractometer with Cu Ka radiation (l ¼ 1.540598Å). The average crystal size of the Pd  nanoparticles was subsequently calculated using the Scherrer equation (D ¼ 0.9l/b cos q, where l ¼ 1.540598Å is the wavelength of the X-ray, b is the full-width at half-maximum height and q is the diffraction angle). 48 Surface morphology of the prepared catalyst was characterized by scanning electron microscopy (SEM) on a Hitachi-SU8010 microscope. Transmission electron microscopy (TEM) analysis on the catalysts was carried out on Tecnai G220 microscope. The surface composition of the IE-Pd/rGO catalyst was analyzed using a ULVAC-PHI Quantera II photoelectron spectroscopy (XPS) system with Al Ka radiation (hn ¼ 1486.6 eV). The thermogravimetric (TG) analysis was carried out on a STA449F3 thermogravimetric analyzer under an O 2 atmosphere from 30 to 800 C at a heating rate of 10 C min À1 . Pd loading of the catalysts was calculated from the residual weight ratio at 800 C of the sample (x Pd ¼ w re M Pd /M PdO , where w re is the residual weight ratio of the sample, M Pd and M PdO are the molecular weight of Pd and PdO, respectively).

Electrochemical measurements
Electro-catalytic activities of the prepared catalysts were measured in a three-electrode cell using a VMP3 electrochemical workstation. The three-electrode electrochemical cell using a glassy carbon (GC) electrode (3 mm in diameter) coated with catalyst serving as the working electrode, a saturated calomel electrode (SCE) and a graphite rod as the reference electrode and the counter electrode, respectively. The catalyst inks were prepared by ultrasonically mixing of catalyst (4 mg), ethanol (0.20 mL, 99 wt%), Naon solutions (0.05 mL, 5 wt%) and deionized water (0.75 mL). Aer evenly dispersed, 10 mL of the suspension was drop dipped onto the GC electrode and subsequently used as the working electrode in measurements. This was repeated once so that it had a loading of 0.56617 mg cm À2 catalyst, and the coating was dried at room temperature for 30 min.
Cyclic voltammetry (CV) measurements were carried out in N 2 -saturated 0.5 M H 2 SO 4 at a scanning rate of 20 mV s À1 . Electrochemical surface area (ECSA) of the catalyst can be calculated from charges (Q) involved in the hydrogen adsorption processes according to the equation of ECSA ¼ Q/0.42 mC cm À2 Â M Pd , 3,49 where M Pd is the Pd loading on the working electrode, 0.42 mC cm À2 is the assuming electrical charge associated with the monolayer adsorption of hydrogen on Pd. Linear sweep voltammetry (LSV) and chronoamperometry (CA) measurements were carried out in a 0.5 M H 2 SO 4 + 0.5 M HCOOH solution. All electrochemical experiments were performed at room temperature.

Results and discussion
Characteristic peaks of (111) and (200) of Pd metal can be detected from the XRD spectrum of the IE-Pd/rGO catalyst as displayed in Fig. 2a, agree well with the PDF card: 03-065-6174. Much boarder (111) peak in the XRD spectrum of the IE-Pd/rGO catalyst than that of the IR-Pd/C catalyst, which was synthesized from a traditional impregnation reduction method, indicates the smaller size of the IE-Pd/rGO catalyst. The board peak around the 2q ¼ 22 is attributed to the X-ray diffraction on the rGO sheets. TEM image on the IE-Pd/rGO catalyst (Fig. 2b) conrms that the Pd nanoparticles are uniformly dispersed on rGO surface with average size of ca. 3.59 nm, agreeing well with that calculated from the (111) peak of the XRD spectrum. It can be also revealed from the TEM images that the Pd nanoparticles are uniformly anchored on the rGO surface with large distance between each two nanoparticles, which is attributed to the diluted Paper distribution of acid groups on the GO sheets. At the same time, the crystal domains within the Pd nanoparticles have an interfringe distance of 0.23 nm (Fig. 2c), close to the lattice spacing of the (111) planes of the face-centered cubic (fcc) Pd crystal, indicating a stable catalytically activity of the IE-Pd/rGO catalyst. 50 To evaluate the Pd loading in the IE-Pd/rGO catalyst, TG analysis was carried out on the IE-Pd/rGO catalyst in O 2  condition. According to the TG curves as shown in Fig. 3, Pd loading of the IR-Pd/C catalyst was calculated to be 23.36 wt%, agreeing well with the Pd : C ratio in the precursors. In contrast, Pd loading of the IE-Pd/rGO catalyst is low to 7.54 wt%, only 1/3 of that of the Pd/C catalyst. This value is slightly higher than desired (ca. 5 wt%) due to the loss of small pieces of GO/rGO sheets during the catalyst fabrication. 0.5 M H 2 SO 4 solution was subsequently used as electrolyte for CV measurements of both the IE-Pd/rGO catalyst and the IR-Pd/C catalyst to evaluate the electrochemical activity area of the catalysts. Although Pd loading of the IE-Pd/rGO catalyst is much lower compared with the IR-Pd/C catalyst, ECSA of the IE-Pd/ rGO catalyst (89.8 m 2 g À1 ) is almost three times higher than that of the IR-Pd/C catalyst according to the CV curves displayed in Fig. 4a. Moreover, capacitance of the IE-Pd/rGO catalyst was signicantly enlarged compared to that of the original rGO, on where no proton adsorption/desorption peak can be detected, due to that the multilayered rGO nanosheets were further stripped and were broken to small pieces. As demonstrated in Fig. 4b, size of the rGO nanosheets were signicantly reduced aer the IE-reduction synthesis. The size reduction on rGO layer would result in higher active surface area for electrochemical reaction. The enlarged surface area also ensures that the nanoparticles are far away from each other and won't aggregate during the fuel cell operation.
Electrochemical FAOR catalytic activity of the IE-Pd/rGO catalyst was further investigated with the linear sweep voltammetry (LSV) curve compared with that of the IR-Pd/C catalyst and the commercial 20% Pd/C (C-Pd/C, Alfa Aesar) catalyst in Fig. 5a. The IE-Pd/rGO catalyst exhibited much high current density during the entire potential sweep from À0.2 V to 1.0 V. Peak FAOR current density on the IE-Pd/rGO catalyst is high than 800 mA mg Pd À1 , which is ca. 4 times higher than that of the IR-Pd/C catalyst as well as that of the C-Pd/C catalyst. This mass activity is among the best reported Pd based FAOR catalysts at the identical condition. 20,37,51,52 Despite the ultra-low Pd loading in the IE-Pd/ rGO catalyst, Pd(0) : Pd(II) ratio in the IE-Pd/rGO catalyst is higher than that of the IR-Pd/C catalyst as demonstrated in the XPS spectra in Fig. 5b. Other than the enhanced FAOR activity, FAOR potential of the IE-Pd/rGO catalyst is also negatively shied by 40 mV compared with the IR-Pd/C catalyst due to the assistant of doped N atoms on rGO surface, which can be conrmed by XPS spectrum of N 1s on the IE-Pd/rGO catalyst in Fig. 5c, resulted from the Ncontaining functional groups, e.g. -NO 2 , on GO surface. [53][54][55][56][57] Specically, specic activity of the IE-Pd/rGO catalyst is calculated to be 0.9 mA cm Pd À2 by considering the mass activity and ECSA, which similar to that of the reported Pd/C catalysts 18 and the IR-Pd/C catalyst, indicating that FAOR process on IE-Pd/rGO catalyst was not altered. Due to the synergistic effect of Pd uniformly dispersion and N atomic doping, stability of FAOR on the IE-Pd/rGO catalyst was signicantly improved. The IR-Pd/C catalyst exhibited an extremely poor stability as shown in the CA curve in Fig. 6. FAOR current density was quickly deceased to ca. 0 within 100 seconds. As a comparison, FAOR current density of the IE-Pd/rGO catalyst was slowly decreased during the entire 3600 s CA measurement. According to the magnied curves shown in the inset of Fig. 6, FA oxidation current density on the IE-Pd/rGO catalyst can be stabilized at ca. 30 mA mg Pd À1 aer the 3600 s CA measurement.

Conclusions
In summary, an ionic exchange strategy was developed for immobilization of Pd nano-particles on rGO support to achieve ultra-low Pd loading for efficient catalysis of formic acid electrooxidation. Pd 2+ ions were exchanged with the protons in the acid functional groups on GO surface and highly dispersed Pd nano-particles were rmly loaded rGO aer mild reduction. Three times higher FA electro-oxidation mass activity was therefore obtained compared with the conventional impregnation method synthesized Pd/C catalyst. More importantly, FA oxidation stability on this IE-Pd/rGO catalyst was also strongly improved due to the strong immobilization of Pd nano-particle and the effect of in situ doped N from the N-containing functional groups on GO.

Author contributions
Jiuxiao Sun and Xingying Luo contribute equally to this work. The manuscript was written through contributions of all authors. All authors have given approval to the nal version of the manuscript.

Conflicts of interest
There are no conicts to declare.